Denatured lysozyme-coated carbon nanotubes: a versatile biohybrid material

Carbon nanotubes (CNTs) are among the most versatile nanomaterials, but their exploitation is hindered by limited dispersibility, especially in aqueous solvents. Here, we show that AP-LYS, a highly cationic soluble derivative of denatured hen egg lysozyme, is a very effective tool for the unbundling and solubilisation of CNTs. AP-LYS proved to mediate the complete and stable dispersion of CNTs at protein: CNT ratios ≥1: 3 (w:w) in very mild conditions (10–20 minutes sonication in ammonium acetate buffer, pH 5.0). Electrophoretic mobility and ζ-potential measurements confirmed that dispersed CNTs were coated by the protein, whereas molecular docking was used to study the interactions between AP-LYS and CNTs. AP-LYS-coated CNTs proved to be a very effective microbial cell-flocculating agent with an efficiency similar to that of chitosan, one of the best available flocculating agents, thus suggesting that this hybrid could find industrial applications in the treatment of wastewaters contaminated by microbial cells, or to remove microbial cells after fermentation processes. Moreover, we exploited the low stability of AP-LYS-coated CNT dispersions in eukaryotic cell culture media to prepare scaffolds with an extracellular matrix-like rough surface for the cultivation of eukaryotic cells.


Results and Discussion
preparation and characterization of MWnt dispersions. The ability of AP-LYS to disperse MWNTs was inspected by sonicating a given amount of MWNTs (typically 3 mg of powder in a final volume of 3 mL) in the presence of increasing concentrations of AP-LYS (from 0.25 to 4 mg/mL) in 10 mM ammonium acetate (AMAC) pH 5.0 for 60 min in an ice-bath, as reported in Table 1. At the end of the sonication, all dispersions were centrifuged at 1000 g for 10 min at 4 °C to remove the undissolved material. As expected, in the absence of AP-LYS, sonication failed to provide stably dispersed MWNTs (sample "a"). As shown in Fig. 1A, in the presence of the lowest concentration of AP-LYS (0.25 mg/mL, sample "b"), the supernatant appeared clear and colorless, identical to the buffer, thus indicating that at this ratio AP-LYS is not able to disperse MWNTs, whereas, at all the ratios AP-LYS:MWNTs above 0.25:1 (samples from "c" to "h"), no sediment was found after centrifugation, and the supernatants appeared black, homogeneous, without any visible aggregate in suspension.
The MWNTs/AP-LYS dispersions (samples "b"-"h") were characterized by UV-Vis absorption spectroscopy, as unbundled CNTs strongly absorb in UV-Vis region. The spectra of the dispersions were similar to those reported in literature for MWNTs dispersions (Fig. 1B).
Very interestingly, with the exception of the sample containing 0.25 mg/mL of AP-LYS (sample "b"), all the other samples showed the same absorbance at 600 nm, thus indicating that all the dispersions contained the same amount of carbon material in solution. This result was in agreement with the absence of pellets after the centrifugation step and suggested that MWNT dispersion was an all-or-nothing process, with a critical AP-LYS:MWNTs ratio between 0.25:1 and 0.33:1. On the basis of these findings we assumed that the concentration of MWNTs in all the samples from "c" to "h" was 1 mg/mL.
All the MWNTs dispersions proved to be very stable over time being essentially unchanged after storage at 4 °C for two years (Fig. S1).  To study the kinetic of the dispersion process, MWNTs powder was sonicated in presence of different AP-LYS concentrations in 10 mM AMAC pH 5.0 and the absorbance at 600 nm was monitored every 10 min. Very interestingly, we found that the dispersion process is essentially complete after 10-20 min of sonication ( Fig. 2A). As previously observed, increasing the amount of AP-LYS:MWNTs ratio did not increase the yield of dispersed MWNTs (Fig. 2B).
Samples from "c" to "h" were characterized by electrophoretic mobility and ζ-potential. All samples migrated toward the negative electrode and the electrophoretic mobility varied from 2.92 ± 0.11 μm s −1 cm V −1 in the sample "c" to 2.34 ± 0.06 μm s −1 cm V −1 , in "h" (Fig. S2). Furthermore, all dispersions showed a positive ζ-potential (Fig. 2C), in the range +30/+37 mV. As the ζ-potential of MWNTs in distilled water is −13 mV 38 , this finding suggests that MWNTs were coated by AP-LYS. Furthermore, ζ-potential values higher than +30 mV indicated that the dispersions were stable and not prone to aggregate 39,40 .
Finally, Transmission Electronical Microscopy (TEM) analyses were performed to inspect the morphology of the samples. As shown in Fig. 2D, TEM images revealed that AP-LYS-coated MWNTs were well dispersed and unbundled.  We then evaluated the ability of AP-LYS to disperse MWNTs at different pH values and in the presence of salt. To this purpose, AP-LYS-coated MWNTs (samples "c"-"h") were prepared at low pH and ionic strength (10 mM AMAC pH 5.0), and then diluted in 10 mM MOPS or 10 mM NaP pH 7.4 in the presence or absence of 150 mM NaCl. Samples were diluted in the appropriate buffer at different nanotube concentrations, from 0.016 to 0.25 mg/mL, centrifuged to remove aggregates, and absorbance at 600 nm was recorded and compared to that of samples diluted in 10 mM AMAC pH 5.0 (Fig. S3). We found that AP-LYS-coated MWNTs were stably dispersed in 10 mM AMAC pH 5.0 in the presence of salt (Fig. S3A), and in 10 mM MOPS pH 7.4 in the absence of salt (Fig. S3B). The presence of NaCl in MOPS buffer induced the complete precipitation of the sample "c" (AP-LYS:MWNTs = 0.33:1), and the partial precipitation of the sample "d" (AP-LYS:MWNTs = 0.5:1) (Fig. S3C). Finally, samples "c" and "d" were not stable, neither in the presence nor in the absence of 150 mM NaCl, in 10 mM NaP pH 7.4 (Fig. S3D,E). These data suggested that the stability of the AP-LYS-coated MWNTs dispersion was influenced by ionic strength, pH, buffer and AP-LYS:MWNTs ratio. Summarizing, AP-LYS-coated MWNTs dispersions were more stable at pH 5 than at pH 7.4 and, at pH 7.4, phosphate induced aggregation more efficiently that MOPS. These results were not unexpected as the net positive charge of AP-LYS, which likely contributes to the stability of the dispersions, is higher at pH 5 than at pH 7.4 36 . Moreover, the anions contained in the buffer could bind to and partially shield the positive charge of the coated MWNTs. Likely, the phosphate di-anion HPO 3 2− (the main species in phosphate buffer at pH 7.4), is more effective than MOPS and chloride at performing the shielding effect.

Molecular docking analysis.
In order to try to understand the molecular basis of the interaction between AP-LYS and MWNTs we performed a docking analysis, as previously described for the interaction between AP-LYS and molybdenum disulfide (MoS 2 ) 37 . We have previously shown that AP-LYS was essentially unfolded in water but it was prone to regain a significant content of helical structure in the presence of trifluoroethanol 36 , an organic solvent widely used to mimic the interaction of proteins and peptides with membranes [41][42][43][44][45][46] . By modelling the interaction of residues 1-18 of lysozyme (Fig. S4), which include the first amphipathic α-helix of native LYS (residues 4-15), we showed that this secondary structure element bound to MoS 2 through Van der Waals and hydrophobic interactions between the hydrophobic face of the helix and the relatively hydrophobic surface of MoS 2 . In particular, we found a ΔG for the adsorption reaction of region 1-18 of about −5.3 kcal/mol (corresponding to a binding constant K = 1.7 10 3 ). With a similar approach we have docked lysozyme region 1-18 to a planar graphene sheet (~74 Å × ~71 Å; 2074 carbon atoms) and to a fragment (~74 Å × ~65 Å; 2074 carbon atoms) of a carbon nanotube with an outer diameter of about 10 nm, the average diameter of the MWNTs used in this study. In the lowest energy complexes, region 1-18 formed an amphipathic helix (spanning residues 4 to 14) with the hydrophobic face in contact with the carbon surface, accordingly to the results obtained with MoS 2 . However, in the case of graphene and of the nanotube fragment, the α-helix contacted the surface with two different orientations, thus providing two alternative complexes with similar energy ( Table 2, Figs 3 and S5).
One of the two complexes was similar to that previously observed in the case of MoS 2 . In this complex, the helix was oriented so that in addition to the residues of the hydrophobic face (Leu8 and Met12) also Glu7 and Ala11 made significant contacts with the carbon surface ( Table 2, Figs 3A and S5A,C). In the second complex, the helix was oriented so that in addition to residues Leu8 and Met12 also residue Arg5, Ala9 and Lys13 (on the opposite side with respect to Glu7 and Ala11) contacted the carbon surface ( Table 2, Figs 3B and S5B,D). In both the orientations, residues 1-3, upstream the helical region, and residues 15-18, downstream the helical region, significantly contributed to binding ( Table 2, Figs 3 and S5). Interestingly, in the case of residues 15-18, in addition to side-chains atoms, also the backbone atoms contributed to binding. This is particularly evident in the case of Gly16 (Table 2) whose peptide bonds were roughly parallel to the surface (especially in models 2), thus allowing amide-π stacking interactions as previously observed in the case of a model alanine dipeptide/ graphene complex 47 . It is interesting to note that the ΔG values for the adsorption process were very similar for the complexes involving graphene and the nanotube fragment, thus indicating that region 1-18 bound with similar efficiency to both planar and curved carbon surfaces (at least with curvature similar to that examined in this study). Furthermore, all the ΔG values were considerably higher in absolute value (−29/−31 kcal/mol) with respect to that observed in the case of the MoS 2 surface. This was an expected consequence of the higher hydrophobicity and polarizability of the aromatic carbon surfaces with respect to the MoS 2 surface. Hypothesizing that the other amphipathic secondary structure elements present in lysozyme contribute cooperatively to the binding, this would explain the strong affinity for carbon surfaces. In general, our analysis supports the hypothesis that AP-LYS could bind to hydrophobic surfaces through amphipathic elements, at least in part corresponding to secondary structure elements of native lysozyme.

AP-LYS-coated MWNTs as microbial cells flocculating agent. Next, as AP-LYS-coated MWNTs
show a cationic nature, we inspected its flocculating ability. Indeed, flocculation is an aggregation process of suspended particles (mineral particles or microorganisms) which eventually undergo sedimentation 48 . This phenomenon can be induced by adding flocculating agents, which cause the aggregation of the particles 48 . As most inorganic particles and microbial cells are anionic, the most effective flocculating agents are synthetic or natural cationic polymers [49][50][51][52] . Thus, we incubated Escherichia coli cultures in the presence of AP-LYS-coated MWNTs (samples "c" and "e") and observed an immediate formation of black flocs, visible to naked eyes, which slowly sedimented (Fig. S6). On the other hand, we did not observe significant flocculation when Escherichia coli cultures were incubated with AP-LYS concentrations in the range 0.1-10 µg/mL (data not shown).
In order to quantify the flocculation efficiency, increasing concentrations of AP-LYS-coated MWNTs (from 0.175 to 5.6 µg/mL) were tested on three bacterial strains which are common sweet-water contaminants, namely Escherichia coli, Salmonella enterica Typhimurium T and Enterococcus faecalis, and on the yeast Saccharomyces www.nature.com/scientificreports www.nature.com/scientificreports/ cerevisiae. Only dispersions "c" and "e" (AP-LYS:MWNTs ratios = 0.33:1 and 1:1, respectively) were used and incubated for 2 or 18 h with the cultures. At the end of incubation, we measured the absorbance at 600 nm of the supernatant (Fig. 4) and the flocculation percentage was calculated as described in section 4.4. The flocculation curves were obtained by plotting the flocculation % as a function of AP-LYS-coated MWNTs concentration. The flocculation assay was performed in the presence and in the absence of 150 mM NaCl to evaluate the effect of ionic strength on the flocculation efficiency.
Dispersions, "c" and "e" showed a very similar behavior. After 2 h of incubation, the efficiency of flocculation, for all the tested microorganisms, ranged between 86 and 96%, using 5.6 µg/mL of AP-LYS-coated MWNTs ( Fig. 4A-D). These values increased to 89-100%, after 18 h of incubation ( Fig. 4E-H). Small differences were observed after 2 h incubation in the presence of NaCl, thus suggesting that salt slows down the flocculation process. In particular, E. coli showed a flocculation efficiency between 87% and 95% after 2 h in the absence of NaCl  www.nature.com/scientificreports www.nature.com/scientificreports/ using either 1.4 or 5.6 µg/mL MWNTs. On the contrary, in the presence of NaCl, 90% of flocculation was observed only using the highest amount of AP-LYS-coated MWNTs (Fig. 4A, green line). After over night sedimentation, flocculation efficiency reached 100% with both AP-LYS-coated MWNTs samples (Fig. 4E, green line). In the case of Salmonella enterica Typhimurium (Fig. 4B,F), a higher flocculation efficiency was found. In the absence of NaCl, 1.4 µg/mL AP-LYS-coated MWNTs were able to flocculate 95% of bacteria after 2 h (Fig. 4B), and 99% after over night incubation (Fig. 4F). The experiments with Salmonella were performed only in the absence of NaCl, as salt induces spontaneous flocculation of the strain (data not shown). AP-LYS-coated MWNTs (5.6 µg/mL) were able to flocculate 90% of E. faecalis after 2 h (Fig. 4C,G). It is intriguing to note that in the case of E. faecalis high flocculation efficiency was observed only after over night incubation, thus suggesting that flocculation of this strain was considerably slower than that of the others. S. cerevisiae had a behaviour similar to that of E. coli, thus demonstrating that AP-LYS-coated MWNTs could flocculate also eukaryotic cells (Fig. 4D,H). It is worth noting that AP-LYS alone, at concentrations up to 10 µg/mL, did not induce the flocculation of E. faecalis and S. cerevisiae, whereas in the case of S. enterica it was able to induce about 20% of bacteria flocculation after 20 h (data not shown). The last finding is not surprising as S. enterica cells were completely flocculated also after the simple addition of 150 mM NaCl, thus indicating that they are particularly prone to aggregate in the presence of ionic compounds.
The presence of flocs in the sediments was confirmed by optical microscopy analysis (Figs 5A and S7). The pellets obtained using 5.6 µg/mL of AP-LYS-coated MWNTs after 2 h of sedimentation were stained using the Live/Dead TM assay and observed by a fluorescence microscope. Dead cells, due to compromised membrane, absorbed the cell impermeant propidium iodide dye and stained red, whereas cells with an intact membrane stained green absorbing the cell permeable dye SYTO 9. All the sediments contained large regular flocs (Figs 5A and S7), characterized by the presence of both live and dead cells in different ratio, depending on the analyzed strain (Fig. S7). A similar behavior was observed in the presence and in the absence of salt (not shown).
Noteworthy, a concentration as low as 0.7 µg/mL of AP-LYS-coated MWNTs was able to induce 100% flocculation of E. coli after over night incubation, (Fig. 4E, black and red lines), which corresponded to an effective concentration of about 0.6 mg/g of dry E. coli cell weight. This value is comparable or lower than those reported for partially de-acetylated-high molecular weight chitosan (MW ≥ 200 kDa), one of the most efficient cell flocculation agent described so far, which is effective at concentrations of about 0.3-5 mg/g of dry cell weight depending on the degree of chitosan de-acetylation [53][54][55] . The high efficiency of partially de-acetylated-high molecular weight chitosan has been explained hypothesizing that the flocculation mechanism is based not only on a nonspecific charge neutralization process caused by the adsorption of the cationic polymer at the surface of the negatively charged cells, but also on a cell "bridging" process due to specific interactions between cells and loops or tails protruding from the adsorbed polymer 54 . A similar mixed mechanism could be operating also in the case of AP-LYS-coated MWNTs. In fact, specific sequences or secondary structure elements present in the AP-LYS molecules, possibly at least in part protruding from the nanotube surface, could be able to bind specifically at the surface of bacterial cell (Fig. S8A,B). It is worth noting that human and chicken lysozymes contain antimicrobial regions similar to cationic antimicrobial peptides, a well known class of antimicrobial agents which kill bacteria by binding to and destabilizing bacterial membranes 56,57 . Taking into account the length of nanotubes -in the range 3-6 µm, i.e. comparable or even longer than that of E. coli cells -it can be hypothesized that AP-LYS-coated nanotubes could effectively bridge bacterial cell as schematically shown in Fig. S8B. On the other hand, free AP-LYS would not be able to induce flocculation due to its low molecular weight (about 14 kDa). In order to www.nature.com/scientificreports www.nature.com/scientificreports/ confirm this hypothesis, E. coli cells flocculated by AP-LYS-coated MWNTs were analyzed by Scanning Electron Microscopy (SEM). Samples were casted on a gold surface, dried at room temperature and imaged without metallization to exploit the high conductivity of MWNTs. Nanotubes were clearly visible as light strings among the cells in the images of both large and small cell aggregates (Figs 5B,C and S9, respectively). The presence of the nanotubes among the cells was also evidenced by AFM (Fig. S10). Therefore, both SEM and AFM confirmed that CNTs were present among bacterial cells aggregated by the addition of AP-LYS-coated MWNTs.
In addition to the flocculating ability, chitosan also possesses antimicrobial activity that depends from its positive charge. Thus, quaternization of amine groups increases the positive charge and makes it less pH sensitive, thus increasing its antimicrobial activity. It is generally assumed that chitosan kills bacterial cells by binding to their surface, damaging the integrity of bacterial membrane and causing the leakage of cells. This can be the case also for AP-LYS-coated MWNTs, in which the high charge and the presence of antimicrobial peptide-like induce www.nature.com/scientificreports www.nature.com/scientificreports/ surface damage and cell permeabilization. This hypothesis is sustained by propidium iodide staining after only 2 h treatment with AP-LYS-coated MWNTs.

AP-LYS-coated MWNTs as scaffolds for eukaryotic cells. Prior to characterize the interaction of eukaryotic cells with AP-LYS-coated MWNTs, the stability of the dispersions in Dulbecco's modified Eagle's
Medium (DMEM), one of the most widely used eukaryotic culture medium, was determined. AP-LYS-coated MWNT dispersions proved to be very unstable in DMEM, in particular in the presence of 10% fetal bovine serum (FBS). In cell culture-treated polystyrene multiwell plates filled with DMEM containing FBS, AP-LYS-coated MWNTs formed large irregular aggregates tightly bound to the bottom of the wells (images not shown). These observations prompted us to verify the possibility to use AP-LYS-coated MWNTs for the preparation of scaffolds for eukaryotic cells, as CNTs have aroused considerable interest in the field of cell culture and tissue engineering since they can form frameworks resembling extracellular matrix (ECM). For example, CNTs functionalized with ECM proteins proved to be particularly promising tools for the preparation of biocompatible scaffolds for cultivation of cell lines difficult to grow, such as stem cells, neurons, osteoblasts and myocytes 10,58 . However, handling of CNTs is made difficult by the necessity to unbundle/disperse them and, successively, to control their assembly in matrix-like insoluble structures. From this point of view the high stability at low ionic strength and moderately acidic pH values of AP-LYS-coated MWNT dispersions, along with their ability to form insoluble aggregates at physiological conditions, provide the possibility to design simple strategies to assemble scaffolds.
Thus, AP-LYS-coated MWNTs was used to coat the bottom of cell culture-treated polystyrene wells, which are characterized by a hydrophilic and negatively charged surface. AP-LYS-coated MWNTs, obtained using all AP-LYS/MWNTs ratios (from 0.33:1 to 4:1), were added to polystyrene plates for 2 h in AMAC at pH 5.0. At the end of the incubation, wells were extensively washed with AMAC and the amount of bound nanotubes was measured by reading the absorbance at 600 nm (Fig. 6A).
All the MWNTs samples were able to coat the bottom of the wells but with different efficiency, depending on the AP-LYS:MWNTs ratio. The sample containing the lowest AP-LYS/MWNTs ratio (sample c) provided the highest amount of bound nanotubes. Increasing the AP-LYS/MWNTs ratio determined a considerable reduction in the amount of bound nanotubes (Fig. 6A). This result could be explained hypothesizing that AP-LYS-coated MWNTs dispersions obtained using lower amounts of AP-LYS (samples "c" and "d") contain not-shielded hydrophobic patches which could contribute to stabilize the binding.
We reasoned that neutralizing the positive charge of the AP-LYS-coated MWNTs layer deposited at the bottom of the well could allow to add a second layer of coated nanotubes trough a layer by layer deposition process. Hence, wells coated with sample "c" were incubated in different conditions: (i) with NaP, (ii) with DMEM or (iii) with DMEM in the presence of 10% FBS. After the removal of the buffer/medium, wells were treated again with sample "c". Figure S11 shows the aspect of wells after the deposition of the two layers. As shown in Fig. 6B the second coating step determined a further increase of the optical density, thus indicating an increase in the amount of bound nanotubes. However, the increase was modest in the wells washed with NaP before the second coating step and significant in the wells treated with DMEM.
In particular, in the wells treated with DMEM containing 10% FBS, the O.D. 600nm were approximately doubled after the second coating step (Fig. 6B), thus indicating that FBS is particularly effective in shielding the positive charge of coated nanotubes. FBS is a very complex mixture of proteins including negatively charged proteins like albumins. These proteins could be adsorbed at the surface of the cationic AP-LYS-coated MWNTs layer, www.nature.com/scientificreports www.nature.com/scientificreports/ thus forming an anionic layer, which could promote the adhesion of a second layer of AP-LYS-coated MWNTs. However, we could not exclude that also specific AP-LYS/serum protein interactions contribute to binding. Very interestingly, the amount of bound nanotubes did not change after incubation of the wells for 96 h at 37 °C in DMEM containing 10% FBS, thus indicating that the AP-LYS-coated MWNTs scaffolds were stable under cell culture conditions (Fig. 6B).
The scaffolds obtained through the two-steps deposition procedure were analyzed by scanning electron microscopy and AFM. Both techniques evidenced the presence of a complex and tangled net of nanotubes (Figs 7 and Fig. S12). In particular, AFM images showed a very irregular surface with several valleys and ridges a feature usually considered well suited for the adhesion of eukaryotic cells.
Finally, two human cell lines, the cancerous HeLa and the immortalized HaCaT cell lines, were cultivated for 24 to 72 h in the wells coated through the two-layers deposition procedure. The Alamar blue cell viability assay showed that the AP-LYS-coated MWNTs scaffold did not influenced cell viability (Fig. S13). Moreover, fluorescence microscopy analysis of the cultures revealed no morphological alterations in both cell lines (Fig. S14). It can thus be concluded that the scaffolds containing AP-LYS-coated MWNTs are well suited for eukaryotic cell cultures.

conclusions
We have demonstrated that AP-LYS, an irreversibly denatured and chemical modified lysozyme derivative, is a very effective tool to prepare long term stable dispersions of carbon nanotubes. The proposed procedure is simple, fast and environment friendly, being carried out without using organic solvents, thus allowing an easy industrial scaling up. It is also worth remembering that hen egg lysozyme is a cheap and widely available protein.
To this regard, it is interesting to compare the efficiency of native LYS and AP-LYS as CNT dispersants. Horn and colleagues, starting from a suspension containing 1 mg/ml of CNTs and 5 mg/ml native LYS, obtained a stable dispersion containing 0.15 mg/ml of CNTs and 2.2 mg/ml of native LYS 31 . Similarly, Nepal and Geckeler using an excess of native lysozyme obtained a stable dispersion containing 0.09 mg/ml of CNTs 30 . On the other hand, AP-LYS allowed to obtain long term stable dispersions containing 1 mg/ml of CNTs, using AP-LYS concentrations lower than that of CNTs. These performances are likely due to the fact that denatured AP-LYS exposes all its hydrophobic residues, whereas native lysozyme only exposes small patches of hydrophobic residues at the surface www.nature.com/scientificreports www.nature.com/scientificreports/ of the native fold. Likely, the intrinsic flexibility and length of the unfolded protein further contribute to favour an extended and strong interaction between AP-LYS and the carbon surface. From this point of view AP-LYS is more similar to random copolymers of amino acids (e.g. co-polymers of lysine and tryptophan 26 ) than to globular proteins. However, differently from copolymers, AP-LYS has a defined weight and sequence. Apart from the direct comparison in terms of yields and effective concentrations, we want to underline that native lysozyme and AP-LYS are not alternative but complementary dispersing agents. In fact, native lysozyme maintains most of its catalytic activity after binding to CNTs 30-32 , therefore, it could be the better suited agent when lytic antibacterial activity is an added value 32 . On the other hand, when catalytic activity is not necessary or even undesirable (e.g. when the aim is to flocculate bacterial cells) AP-LYS is better suited. Furthermore, AP-LYS itself is not just a dispersing agent, but it also adds new functionalities to CNTs. The high positive charge and the presence of bioactive antimicrobial peptide-like regions make AP-LYS-coated CNTs a very effective tool for microbial cell flocculation with an efficiency similar to that of chitosan, a benchmark in the field. Moreover, we have shown that precipitation in eukaryotic cell culture media allows to prepare stable scaffolds with high surface roughness. This could be useful in the cultivation of cell lines with particular requirements, such as neurons and myocytes. We want also to underline that AP-LYS-coated CNTs could be further covalently modified by exploiting several very well-known protein-modification strategies 59 , thus expanding the potential applications of this new bioconjugate. Finally, it is worth noting that, similarly to lysozyme(s), other disulfide rich proteins -e.g. pancreatic type ribonucleasescan be reduced to obtain denatured yet soluble proteins 60 , thus suggesting that our approach could pave the way toward a new family of biohybrid materials.
MWNTs dispersions were prepared in batches of 3 mL in 10 mM ammonium acetate pH 5.0 by mixing 3 mg of MWNTs powder (Sigma-Aldrich) and different AP-LYS concentrations (from 0.25 to 4 mg/mL), using a medium power tip sonicator (Sonics, Vibra cell VC505). Samples were sonicated in an ice bath for 10-60 min. The suspensions were centrifuged at 1000 g for 10 min at 4 °C. Supernatants were collected and stored at 4 °C. Supernatants were labelled "a"-"h" as detailed in Table 1. characterization of the dispersions. The UV-Vis spectra of samples "a"-"h", prepared as described in the previous section, were recorded using an UV-Vis spectrophotometer Cary 100 Scan using a 1 cm quartz cell.
Transmission electron microscopy (TEM) measurements were performed on a JEOL JEM 1011 microscope operating at an accelerating voltage of 100 KV. A droplet of the MWNTs was directly deposited on a microscope grid and analyzed.
Electrokinetic analysis and ζ-potential were carried out in folded capillary cells using a Malvern Zetasizer Nano-ZS system equipped with a 633 nm He-Ne laser. All measurements were conducted at 25 °C. Docking of lysozyme fragment 1-18. The interaction of fragment 1-18 of lysozyme with graphene and CNT surfaces was modelled by using a Monte Carlo energy minimization strategy as previously described for a MoS 2 monolayer 37 . All calculations were performed using the ZMM-MVM molecular modelling package (ZMM Software Inc. [http://www.zmmsoft.com]) which has already proved useful for the modelling of several complexes of different nature and size [61][62][63][64][65] . The model complexes included lysozyme fragment 1-18 and a fragment either of a planar graphene sheet or of a carbon nanotube with an outer diameter of about 10 nm and a chirality index (73, 73) generated by the TubeASP, carbon nanotube generation applet (http://www.nanotube.msu.edu/tubeASP/). Both carbon surfaces included 2074 carbon atoms with approximate dimension ~74 Å × ~71 Å in the case of the planar surface and ~74 Å × ~65 Å in the case of the CNT fragment. Both the graphene and CNT fragments were frozen throughout the simulation process.
Initial structures of the lysozyme fragment were prepared using PyMOL (DeLano Scientific LLC, https://www. pymol.org/) and DeepView -Swiss-PdbViewer 66 . Two initial structures were modelled, a completely helical and a completely extended structure. Each structure was used to generate eight starting manually prepared complexes for each of the two carbon surfaces: fragment 1-18 was placed parallel to the surface with the termini of the peptide pointing toward either the zigzag or the armchair edges of the carbon surface, hence the peptide structure was rotated by steps of 90°. Each of the sixteen models (eight for the planar and eight for the curved surface) www.nature.com/scientificreports www.nature.com/scientificreports/ was used as starting point for a Monte Carlo trajectory. Trajectories were stopped when no energy decrease was observed for 1000 minimization cycles. Energy calculations included an implicit water solvation component calculated as previously described 67,68 .
For each optimized complex total peptide/carbon surface binding energies were calculated by summing the residue/carbon surface binding energies provided by the ZMM Software. Fragment 1-18 alone was also modelled (Fig. S4B) in order to calculate a theoretical change in Gibbs free energy ΔG for the adsorption reaction: peptide (aq.) + carbon surface (aq.) = peptide/carbon surface complex (aq.) ΔG was calculated by the equation: where E complex is the energy of the minimized carbon surface/peptide complex; E C-surface is the energy of the carbon surface alone; E peptide is the energy of the peptide minimized in the absence of the carbon surface.
flocculation. Flucculation was determined as previously described 54  Flocculation experiments were conducted at room temperature and each experiment was repeated three times. The LIVE/DEAD Bacterial Viability Kit (BacLightE) was used to determine the viability of bacteria after incubation with MWNT. Staining was performed according to the manufacturer instructions. The flocs were placed on microscope slides and covered with a coverslip. Images were captured using an Olympus DP70 digital camera equipped with Olympus U-CA Magnification Changer (magnification 100×) and processed with Image Analysis Software (Olympus) for minor adjustments of brightness, contrast and color balance and for creation of merged images. Exposure times were in the range between 50 and 200 ms.
Ap-LYS-coated MWnts binding to polystyrene plates. Fifty microliters of AP-LYS-coated MWNTs samples "c"-"h" were added to cell culture-treated polystyrene plates (96-well, Corning). After 2 h incubation at 37 °C, wells were washed with 10 mM AMAC pH 5.0 for three times and the degree of coating of polystyrene wells was measured by reading the absorbance at 600 nm in a multiwell reader (Synergy HTX Multi-Mode Reader-BIOTEK). All the absorbance values were corrected subtracting the absorbance of untreated wells.

Layer by layer deposition of Ap-LYS-coated MWnts. Polystyrene wells treated with AP-LYS-coated
MWNT sample "c" as described in the previous section, after extensive washes with AMAC buffer (10 mM, pH 5.0), were incubated for 60 min at 37 °C in different conditions: (i) with 10 mM NaP, pH 7.4; (ii) with DMEM; (iii) with DMEM in the presence of 10% FBS. After removal of NaP and DMEM, wells were incubated again with 50 µL of sample "c" for 1 h at 37 °C. The degree of coating of polystyrene wells was measured by reading the absorbance at 600 nm at the end of the preparation and after 96 h incubation at 37 °C in DMEM containing 10% FBS. cell cultures. The Alamar Blue assay was used to assess cell viability based on the reduction potential of metabolically active cells. Human immortalized keratinocytes (HaCaT) and human cancer epithelial cells (HeLa) were cultivated in the wells coated with two layers of MWNTs (sample c) in complete medium (DMEM containing 10% FBS, 2 mM L-glutamine and antibiotics) at 37 °C in a humidified atmosphere containing 5% CO 2 . At the end of incubation, AlamarBlue ® reagent (Invitrogen) was added in each well and incubated for 3 h at 37 °C.
The fluorescence intensity was measured at an emission wavelength of 585 nm and an excitation wavelength of 570 nm using a plate reader (Synergy HTX Multi-Mode Reader-BIOTEK). Cell survival was expressed as the percentage of viable cells grown on the nanotube scaffolds compared to controls. Each sample was tested in three independent analyses, each carried out in triplicate. Cell viability was expressed as mean values ± SD. Significance was determined by Student's t-test at a significance level of 0.05. In order to analyze the morphology of HaCaT and HeLa cells grown on the CNT scaffolds the cells were stained with the viable, cell permeable fluorescent stain fluorescein diacetate (FDA). FDA stock solution was prepared in acetone at 5 mg/mL. Cells were seeded in 96-well plates coated by MWNTs dispersion (sample c) at a density of 1 × 104/well and then grown at 37 °C for 24 h. Cells were treated with FDA (1 µg/mL) in DMEM without FBS for 5 minutes in the dark. After removing the staining solution, DMEM was added to the cells. Cells were analyzed by a Leica DMi8 fluorescence microscope (magnification 20×) using a FITC filter. Typical acquisition time was 100 ms. The images were captured using a Leica DFC 310 FX digital camera and processed by using the analysis software supplied by the manufacturer.